User talk:Kebumen

Stages of production process tile

Kebumen - central java - the Indonesia industry is very good. Raw materials in the form of clay obtained with the extraction of rice with the hoe to a depth up to one meter. At the top of the deep as 25 centimeters removed because oxygen-containing organic substances.

* Preparation of materials (clay). Processing of the raw material mixed sand suntil evenly then put in the engine molen. This process aims to destroy grain-grain rough ground become more finely done so repeatedly to get the land that is completely smooth. Then the land is inserted in the machine or corkscrew opium aims to reduce the pore-pore kekedapan determine the future of tile water. In the land of this engine is driven by a cylindrical tube through incentive systems with a shovel and clay will be out through a small hole so it's going opium den. Hole out land quadrangular with size 10 cm x 25 cm. then in a table-cut piece of land cut quadrangular with a certain size in accordance with the type of tile that will be produced.

* Printing Stage is the stage of printing the form of a tile from keweh. inserted in a hand press machine has been given a lubricant (nyamplung oil or coconut oil) to keweh not sticky on the printing machine and makes the tile more finely. Then on the tray edge tile to be made by using the excess

* Drying Drying process is done gradually. At the beginning of the tile diangin-anginkan for a few days (5-7 days). When drying the first phase is considered adequate (color slightly whitish), and the next stage is the season in the sun for 6-8 minutes until the yellow whitish.

* Burning Burning is the process of production from the end of the tile which can determine the quality and quantity of production tile. At first tile that has been inserted in the dried tobong (kiln) until the appropriate size of the full-size tobong. At the beginning of the heating using a small fire for about 90 minutes to improve the drying process. In the beginning of smoke-colored dusky, the white smoke after the fire and be enlarged up to 5 hours, the tile color will appear reddish and then raised the temperature up to a maximum level for about 20 hours. Burning took place during this 4-5 days. After that, refrigerated for 2 days.

* demolition and sorting (selection) After the cooling process is complete, the tile is removed from tile and sorting is done based on the criteria of color and integrity of the surface of tile.